Over deze norm
1.1 This test method covers direct determination of the proportion by mass of individual phases in portland cement or portland-cement clinker using quantitative X-ray (QXRD) analysis. The following phases are covered by this standard: alite (tricalcium silicate), belite (dicalcium silicate), aluminate (tricalcium aluminate), ferrite (tetracalcium aluminoferrite), periclase (magnesium oxide), gypsum (calcium sulfate dihydrate), bassanite (calcium sulfate hemihydrate), anhydrite (calcium sulfate), and calcite (calcium carbonate).
1.2 This test method specifies certain general aspects of the analytical procedure, but does not specify detailed aspects. Recommended procedures are described, but not specified. Regardless of the procedure selected, the user shall demonstrate by analysis of certified reference materials (CRM's) that the particular analytical procedure selected for this purpose qualifies (that is, provides acceptable precision and bias) (see Note 1). The recommended procedures are ones used in the round-robin analyses to determine the precision levels of this test method.
Note 1—A similar approach was used in the performance requirements for alternative methods for chemical analysis in Test Methods C114.
1.3 The values stated in SI units shall be regarded as the standard.
1.4 This standard does not purport to address all of the safety concerns, if any, associated with its use. It is the responsibility of the user of this standard to establish appropriate safety and health practices and determine the applicability of regulatory limitations prior to use. For specific hazards, see Section 9.
|Nederlandse titel||Standard Test Method for Determination of the Proportion of Phases in Portland Cement and Portland-Cement Clinker Using X-Ray Powder Diffraction Analysis|
|Engelse titel||Standard Test Method for Determination of the Proportion of Phases in Portland Cement and Portland-Cement Clinker Using X-Ray Powder Diffraction Analysis|